Influence of surface stress on elastic constants of
Physica E 53 (2013) 217–222
Contents lists available at SciVerse ScienceDirect
journal homepage: www.elsevier.com/locate/physe
Inﬂuence of surface stress on elastic constants of nanohoneycombs
Qiang Chen a, Nicola Pugno b, Zhiyong Li a,n
Biomechanics Laboratory, School of Biological Science and Medical Engineering, Southeast University, 210096 Nanjing, PRChina
Department of Civil, Environmental and Mechanical Engineering, University of Trento, 38123 Trento, Italy
H I G H L I G H T S
G R A P H I C A L
The regular hexagonal honeycomb is
not isotropic but orthotropic.
The competition between the surface residual stress and the surface
The surface residual stress dominates the surface effect when the
cell-wall thickness t o15 nm while
the surface elasticity does when
Summary: Comparision of shear modulus predicted by different considerations, i.e., without surface
effect, only surface elasticity, both surface elasticity and surface residual stress.
art ic l e i nf o
a b s t r a c t
Received 10 January 2013
Received in revised form
12 April 2013
Accepted 1 May 2013
Available online 9 May 2013
Surface effect on the four independent elastic constants of nanohoneycombs is investigated in this paper.
The axial deformation of the horizontal cell wall is included, comparing to the Gibson's method, and the
contributions of the two components of surface stress (i.e. surface residual stress and surface elasticity)
are discussed. The result shows that the regular hexagonal honeycomb is not isotropic but orthotropic.
An increase in the cell-wall thickness t leads to an increase in the discrepancy of the Young's moduli in
both directions. Furthermore, the surface residual stress dominates the surface effect on the elastic
constants when t o15 nm (or the relative density o0.17), which is in contrast to that the surface
elasticity does when t 415 nm (or the relative density 40.17) for metal Al. The present structure and
theory may be useful in the design of future nanodevices.
& 2013 Elsevier B.V. All rights reserved.
A B S T R A C T
Due to the existence of a surface, surface effect resulting in an
excess free energy per area , produces an important inﬂuence on
the mechanical properties of nanostructures when the structure's
size comes down into nanoscale (less than 100 nm) . At present,
a huge number of works studies the mechanical behaviors of rod- or
wire-like nanostructures for potential applications in micro- or nanoelectromechanical systems by performing experiments  or popular
numerical method—molecular dynamics simulations , such as
elasticity , fracture , buckling  and plasticity . In theoretical
Corresponding author. Tel/fax.: +862583792620.
E-mail address: [email protected] (Z. Li).
1386-9477/$ - see front matter & 2013 Elsevier B.V. All rights reserved.
aspect, models are often treated as structures with bulk core and
surface shell, i.e., so-called core–shell model [9,10], or composite
model . These works provide deep insights of the mechanisms of
surface effect on mechanical properties of the tiny structures.
Not conﬁned by the nano-wire-structures, nanoporous structures have also drawn considerable attention for the future
applications, e.g. catalysts, molecular sieves. Starting from fabricating technology, nanochannel  and mesoporous structures
 were ﬁrstly developed by chemical methods, and the mechanical properties of the nanoporous materials have been investigated
recently. Indeed, due to the high surface/volume ratio of the
nanoporous structures, the formula of macroporous materials
loses their validity, and the surface effect has to be included. For
example, by incorporating the surface effect into the continuum
mechanics of the composite materials, the elastic constants of the
Q. Chen et al. / Physica E 53 (2013) 217–222
nanoporous materials with uniformly distributed cycle channels
and the Young's modulus of the regular nano-foams were studied
[14–16]. All of the results show that the nanoporous structures can
be stiffer (positive surface effect) or softer (negative surface effect)
than their parent materials, which are dependent on the crystal
orientations. Zhang and Wang  presented a theory to study the
surface energy on the yield strength of nanoporous materials,
basing on the traditional micromechanics. In particular, for irregular nanoporous materials, the Hall–Petch relationship, which
states that the materials' strength is proportional to the reciprocal
of the square root of their grain size (i.e., materials' yield strength
increases as their grain size decreases), is often employed to
predict the effective materials' strength [18,19], and the classical
power law to calculate the mechanical parameters of foam
materials is modiﬁed according to the effective mechanical
strength. But it is worth mentioning that an inverse Hall–Petch
relationship may appear in nanostructures because of sufﬁciently
small grain size, and several reasons are considered to contribute
to this phenomenon . Furthermore, the effect of surface stress
on the plastic deformation of nanoporous or nanocomposite
materials was formulated by a micromechanical framework .
Recently, inspired by the hierarchical structures of natural materials, which span from nano- to macro-scale, a hierarchical foam or
honeycomb taking the surface effect of nano-scale sub-structures
into account was developed by the authors [22–24].
As discussed before, the elastic constants of the nanoporous
materials with uniformly distributed cycle channels and regular
nano-foam have been studied based on a continuum mechanics,
but the surface effect on the elastic properties of the hexagonal
honeycomb (or nanoporous materials with uniformly distributed
hexagonal channels, Fig. 1) is not investigated yet. To this end, here
we developed a relevant theory for the nanohoneycombs, and
compared the results with different theories. Moreover, the
inﬂuences of the cell-wall thickness and the relative density on
the four independent elastic constants of regular Al nanohoneycombs were studied. Besides, we have to point out that the
hexagonal unit cells of the structure is stable , and the
curvature induced by the residual surface stress  is neglected;
this is because the smallest size of the cell walls discussed in this
work is 5 nm, over which the mechanical properties of the cell
walls are close to those of their bulk counterparts [5,11].
2. Surface stress
Surface effect was ﬁrstly introduced by Gibbs  in the sense of
thermodynamics of surfaces, and a keystone in the theory is about
the surface free energy. As for the surface stress caused by the
surface free energy, it is generally expressed as :
τij ¼ γδij þ ∂γ=∂εij , where, γ is the surface excess free energy, δij is
the Kronecker delta, and εij is the strain tensor. For the elastic case,
τij can be rewritten as : τij ¼ τ0ij þ K ijkl εkl , where, τ0ij is the surface
residual stress tensor, and K ijkl is the stiffness matrix. Due to the
structural deformation inducing the change of surface curvature,
the surface stress will produce a distributed force perpendicular to
the structural surface, and the distributed force is easily formulated by the general Young–Laplace equation : Δsij ni nj ¼ ταβ κ αβ
(i, j¼1,2,3 and α, β¼1, 2), Δsij is the stress difference across the
structural surface, ταβ and κ αβ are the surface stress tensor and
surface curvature tensor, respectively. Then, for a one-dimensional
nanostructure, the distributed force along its longitudinal axis can
be expressed as qðxÞ ¼ ΔsðxÞ ¼ Hw″, where, H ¼ 2τW for rectangular cross-sections, w″ is the approximate curvature under small
deformation, and W is the width of the cross-sections. Plus,
because of the small displacement, H can be written as
H 0 ¼ 2τ0 W . In the following sections, the distributed force
qðxÞ ¼ 2τ0 Ww″ will be employed to derive the elastic constants of
It is worth mentioning that surface stress is composed of two
parts from the expressions τij : The ﬁrst is contributed by the
intrinsic surface residual stress and the second by the structural
deformation (or surface elasticity); interestingly, the surface elastic modulus in the second part can be positive or negative; this is
due to the fact that a surface cannot exist without the bulk, and
the total energy (bulk and surface) needs to satisfy the positive
deﬁniteness condition . As for their contributions to the
structural behavior, both the surface elasticity and surface residual
stress have signiﬁcant inﬂuences on the vibrational behavior of
micro- or nano-beams . In particular, the surface residual
stress (or residual strain) prevails on the plastic behavior of the
nanoporous and nanocomposite materials  compared to the
surface elasticity, and the theoretical frame based on strain
gradient theory also supports that residual elastic strain gradient
(or residual stress) effect is signiﬁcant in the elastic deformation of
small-scale structures , and more, the residual stress ﬁeld
considerably affects the effective Young's modulus of Al nanowire
. Here, addressing their inﬂuences on the Al nanohoneycomb,
we will discuss this point in Section 5.
3. Elastic constants
3.1. Young's modulus in 1-direction and Poisson's ratio ν12
The total deformation in 1-direction includes two components:
the bending deﬂection of inclined cell walls (B & C) and the axial
deformation of horizontal cell wall A (Fig. 2(a)). On the one hand,
according to the classical Euler formula for pure-bending structures, the modiﬁed result by surface effect of the cell wall is
expressed as :De w″ ¼ H 0 w′′, where w(x) is the cell wall deﬂection, and De ¼ Dð1 þ 6lin =tÞ [5,32], in which De is effective ﬂexural
rigidity of cell walls, D ¼ EWt 3 =12 is ﬂexural rigidity without
surface effect, and lin ¼ Esur =E with surface Young's modulus Esur
is the materials' intrinsic length [22–24,32]. Then, the differential
equation is solved as, wðxÞ ¼ A1 e−kx =k þ A2 ekx =k þ A3 x þ A4 with
boundary conditions wð0Þ ¼ w′ð0Þ ¼ w′ðLÞ ¼ 0, w‴ðLÞ ¼ −P 1 =De , in
which k ¼ H 0 =De and P 1 ¼ s1 WLcos2 θ. Substituting the boundary
conditions into wðxÞ, we immediately obtained the four integral
tanh þ 1 ;
tanh −1 ;
and the bending deﬂection wðxÞ of the cell walls (B & C) is
Fig. 1. Regular hexagonal nanohoneycomb.
Q. Chen et al. / Physica E 53 (2013) 217–222
Fig. 2. Unit-cell deformations in (a) 1-direction and (b) 2-direction of nanohoneycombs.
the maximum displacement located at x¼ L, and it is formulated as
tanh ⋅ðcosh β−1Þ−sinh β
with β ¼ kL
δb1 ¼ 0 1 þ
On the other hand, the axial displacement of the cell wall A is
2P 1 h
where, d ¼ dð1 þ 2lin =tÞ  is the effective tensile stiffness of cell
walls, in which d ¼ EA is tensile stiffness without surface effect.
Finally, the total displacement Δ1 is obtained as
Δ1 ¼ δb1 cos θ þ δa1 ¼
P 1 Lcos θ
f 1 ðβÞ
and the Young's modulus in the 1-direciton is derived:
h=L þ sinθ
f 2 ðβÞ
P 2 ¼ s2 Wðh þ Lsin θÞsin θ:
so the displacement Δ2 is expressed as
Δ2 ¼ δb2 sinθ ¼
P 2 Lsin θ
f 2 ðβÞ
s2 WLðh=L þ sinθÞsin2 θ
f 2 ðβÞ
H 0 cosθ
Thus, the Young's modulus in the 2-direciton is derived:
ðh=L þ sinθÞsin2 θ
ðh=L þ sinθÞsinθ f 2 ðβÞ
f 1 ðβÞ
ðδ1 cosθ þ δa1 Þ=ðh þ LsinθÞ
and the corresponding Poisson's ratio ν21 is expressed as
ν21 ¼ −
correspondingly, the Poisson's ratio ν12 is also obtained:
ν12 ¼ −
Then, the strain in the 1-direction is calculated:
s1 WLcos3 θ
f 1 ðβÞ
h þ Lsinθ
H ðh=L þ sinθÞ
and the strain in the 2-direction is calculated:
tanh ⋅ðcosh β−1Þ−sinh β þ
f 1 ðβ Þ ¼ 1 þ
Ecos θ L
1 þ 2lin =t
of the inclined cell walls (B & C), and their boundary conditions are
identical with those of the 1-direction. Then, the displacement δb2
is similar as Eq. (2) but with a different load P2, i.e.,
δb cosθ=ðh þ LsinθÞ
¼ 2 b
ðh=L þ sinθÞsinθ
Different from Eq. (7), Eq. (12) is the same as that reported in
Ref. , and this is due to no axial displacement of cell walls in
the 2-direction. Thus, the regular hexagonal honeycomb is not an
isotropic structure any more, but the reciprocal relationship
E1 ν21 ¼ E2 ν12 still holds, that is to say, the structure is orthotropic.
3.3. Shear modulus
tanh ⋅ðcosh β−1Þ−sinh β
f 2 ðβÞ ¼ 1 þ
Apparently, f 1 ðβÞ 4f 2 ðβÞ, the Poisson's ratio ν12 is less than 1 for
regular hexagonal honeycombs of which ν12 is a constant in .
This is because the axial deformation is neglected due to its
smallness compared with the bending deﬂection, when the cellwall thickness is small; however, the difference between these two
methods tends to be larger as t=L (or relative density) increases,
which will be shown later.
3.2. Young's modulus in 2-direction and Poisson's ratio v21
Likewise, we ﬁnd that the displacement of the cell walls under
the 2-direction stress is only contributed by the bending deﬂection
Deformation of cell walls under shear load in honeycombs is
more complex than those under normal stresses in the two
directions discussed above. The shear deformation includes the
rotation angle ϕABC of the joint of cell walls A, B, C, and the vertical
translation δA of the point a, see Fig. 3. In Fig. 3(a), a, b, c denote the
middle points of the cell walls A, B, C, respectively. At point a, there
is a vertical displacement and rotation, whereas, at points b, c, only
rotation exists, because of the structural anti-symmetry; therefore,
the structure could be simpliﬁed as Fig. 3(b) and the total
displacement at point a is 
Δ12 ¼ ϕABC h=2 þ δA
On the one hand, for the rotational angle ϕABC , reconsidering the
expression of wðxÞ but with different boundary conditions of the
cell wall B according to Fig. 3(b), i.e., wð0Þ ¼ w ðL=2Þ ¼ w″ð0Þ ¼ 0,
Q. Chen et al. / Physica E 53 (2013) 217–222
Fig. 4. Unit cell of nanohoneycombs with (a) cylindrical nano-channel and
(b) hexagonal nano-channel.
Fig. 3. Deformation of cell wall under shear load. (a) Representative element
deformation; (b) simpliﬁed structure.
w‴ðL=2Þ ¼ M=De , where M ¼ Sh=4 and S ¼ 2s12 WLcos θ, we ﬁnd
the four integral constants:
A1 ¼ − e sinh
; A2 ¼
A3 ¼ − e ⋅ ;
D k kL
A4 ¼ 0; thus, wðxÞ is expressed as
furthermore, the rotation angle ϕABC ¼ w′ðL=2Þ is obtained:
On the other hand, the vertical translation δA is calculated from
the existing formula of the cantilever structure :
with β′ ¼
then, substituting Eqs. (15) and (16) into Eq. (13), the shear
displacement is obtained:
Sh h β
2H 0 2L 2
thus, the shear strain is calculated:
L ⋅cos θ
¼ s12 h
ðh þ Lsin θÞ=2
−1 þ cosh β′ 1− tanh β′
Finally, the shear modulus is obtained:
þ sin θ
4. Example and discussion
4.1. Comparison of shear modulus of nanohoneycombs with different
In this part, we compare our prediction on the shear modulus of
the present structure (Fig. 4(a); θ ¼ 30o and h=L ¼ 1) with that of the
other similar structure (Fig. 4(b)) presented in the literature  under
the identical conditions of constant porosity 0.2 (or relative density
0.8), side length L and out-of-plane depth of unit cells (Fig. 4). Other
parameters are set as below: First, according to the porosity 0.2 and
the geometry in Fig. 4(a), we obtain the relationship between the side
Fig. 5. Comparison of shear moduli predicted by different methods. Note: The
shear moduli of the nanohoneycombs are normalized by those of the honeycombs
without surface effect.
length L and cell-wall thickness t, i.e., L ¼ 1:045t; likewise, for the
structure in Fig. 4(b), we ﬁnd L ¼ 2:459R; if the pore radius R varies
from 1 nm to 30 nm and then t from 2.353 nm to 70.593 nm; second,
we also use the data of Al presented by Miller and Shenoy , namely,
the bulk Young's modulus E of Al is 89.392 GPa, the surface Young's
modulus Esur on surfaces of [1 1 1] and [1 0 0] crystal orientations for
plates are 5.1811 N/m and −7.9146 N/m, respectively, and the surface
residual stress τ0 on the two surfaces are 0.9096 N/m and 0.5682 N/m,
In Refs. [14,24], the surface elasticity is only considered; therefore,
the inﬂuence of the surface residual stress can be evaluated thanks to
the inclusion of both the surface elasticity and surface residual stress
by comparing the two cases. The results are reported in Fig. 5.
Fig. 5 shows that surface effect on the shear modulus decreases as
the cell-wall thickness t increases. The present method agrees very
well with the result from Ref. , and this explains that the inﬂuence
of the surface residual stress is very weak in the elastic deformation of
nanohoneycombs when the relative density is 0.8. Moreover, the
prediction is comparable to the result from Ref. , even though our
result shows a slightly greater inﬂuence on the [1 1 1] orientation
surface; this is induced by their different geometries and other effects
(such as the shear effect in the bending of cell walls). Moreover, it is
noted that the negative surface Young's modulus softens the shear
behavior of the nanohoneycomb.
4.2. Competition between surface elasticity and surface residual
Let us continue the previous example, but the cell-wall thickness t
varies from 5 nm to 29 nm, and the side length L is maintained as a
constant (100 nm); thus, the corresponding relative density ranges
Q. Chen et al. / Physica E 53 (2013) 217–222
Fig. 6. Comparisons of four elastic constants on the surfaces of [1 1 1] and [1 0 0] orientations, inﬂuenced by only surface elasticity (the black and red curves) or both surface
elasticity and surface residual stress (the green and blue curves). (a) Young's moduli in the 1-direction; (b) Young's moduli in the 2-direction; (c) Poisson's ratio ν12; (c) Shear
moduli. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
from 0.06 to 0.31. Like the comparison of the shear modulus, two cases
are considered: One is only considering the surface elasticity, and the
other both surface elasticity and surface residual stress, the results are
reported in Fig. 6, in which EG and GG are Young's modulus and shear
modulus calculated by the Gibson's method, respectively .
In Fig. 6, an increase in cell-wall thickness generally results in a
decrease in the surface effect on the four independent elastic
constants. If the surface elasticity is only considered, the normalized
Young's moduli and shear modulus are enhanced for positive Esur and
reduced for negative Esur as cell-wall thickness decreases, which
again softens the mechanical behavior of the nanohoneycomb. E1 =EG
of the two surfaces approach a value less than one due to the
inclusion of the axial deformation of horizontal cell walls (black and
red lines in Fig. 6(a)); whereas, E2 =EG or G12 =GG approach unity,
which is the result by the Gibson's method (black and red lines in
Fig. 6(b and d)). However, the surface elasticity does not inﬂuence the
Poisson's ratio ν12 at all (black line and red circle in Fig. 6(c)).
On the other hand, if the surface elasticity and surface residual
stress are both included, the surface residual stress plays much
more important roles when the cell-wall thickness is less than
15 nm (or relative density o0.17); this is because the cell walls B &
C in Fig. 3 are similar as one-end clamped and one-end guided
structures, and in this case, the distributed force induced by the
surface residual stress produces an opposite deﬂection to that by
the external normal load, thus, δbi (i ¼1,2) decreases and τ0
strengthens nanohoneycombs; so, the two Young's moduli are
improved and greater τ0 results in greater Young's modulus (green
and blue lines in Fig. 6(a and b)); different from the surface effect
on the other constants, the surface effect on the Poisson's ratio is
much weaker (green and blue lines in Fig. 6(c)); for the shear
modulus, different from the cell walls B & C, the cell wall A is
equivalent as a cantilever structure, so the distributed force
produces a consistent deﬂection to that by the external shear
load, therefore, δA increases and τ0 softens nanohoneycombs
(green and blue lines in Fig. 6(d)). In the end, the elastic constants
inﬂuenced by both surface elasticity and surface residual stress on
the same crystal surface tend to those inﬂuenced only by the
surface elasticity when cell-wall thickness increases after 15 nm.
Therefore, we can conclude that the surface residual stress
dominates the surface effect when t o15 nm (or relative densityo0.17), while the surface elasticity dominates when t 415 nm
(or relative density 40.17). At this point, it is different from the
conclusion by Feng et al. , which reported that the surface
residual stress has a weaker inﬂuence on the effective elastic
constants than the surface elasticity; this is because in that work
they considered a large constant relative density 0.35 (4 0.17 ),
and the weaker inﬂuence of the surface residual stress is also
observed in Fig. 5 under the larger constant relative density 0.8
4.3. Elastic modulus of Al nanohoneycombs
Here, we again use the above set of surface properties, the
variable t, constant L. Addressing the four independent elastic
constants, the comparison between the results of nanohoneycombs with both surface elasticity and surface residual stress and
macrohoneycombs (Gibson's method) are reported in Fig. 7 versus
relative density. For the two Young's moduli and shear modulus in
Fig. 7(a, b, d), the normalized values can be referred to those in
Fig. 6(a, b, d). In Fig. 7(c), the results of the Poisson's ratio predicted
by different methods are compared, and the present method
considering the axial deformation of horizontal cell walls is
between the FEM  (Timoshenko beam theory) result and unity,
which is formulated by the Gibson's method (Euler beam theory).
Q. Chen et al. / Physica E 53 (2013) 217–222
Fig. 7. Young's moduli of nanohoneycombs in the (a) 1-direction and (b) 2-direction on the surfaces of [1 1 1] and [1 0 0] orientations; (c) comparison of Poisson's ratio by
different methods, note that FEM (TB) denotes Timoshenko-beam element in ﬁnite element method; (d) shear moduli of nanohoneycombs on the surfaces of [1 1 1] and
[1 0 0] orientations.
In this paper, we have calculated the elastic constants of nanohoneycombs inﬂuenced by the surface effect (surface residual stress and
surface elasticity), and different from the Gibson's method, the axial
deformation of the horizontal cell wall is included. The result shows
that the regular hexagonal honeycomb is not isotropic but orthotropic,
and as the cell-wall thickness t increases, the discrepancy of the
Young's moduli in two directions increases. Meanwhile, the surface
effect plays a vital role when t is a few nanometers; when to15 nm,
the surface residual stress dominates the surface effect on the elastic
constants of metal Al nanohoneycombs, otherwise (i.e. t415 nm), the
surface elasticity does. Finally, the nanohoneycomb and present theory
could be important and useful in the design of nanosieves or other
This study was partially supported by the National 973 Basic
Research Program of China [No. 2013CB733800] and the National
Natural Science Foundation of China (NSFC) (No. 11272091) to ZL. The
research related to these results has received funding from the
European Research Council under the European Union's Seventh
Framework Programme (FP7/2007–2013)/ERC Grant agreement nu
 (ERC StG Ideas 2011 BIHSNAM on “Bio-inspired hierarchical
super nanomaterial's’ to NP).
 J.W. Gibbs, The Scientiﬁc Papers, J.W. Gibbs, Longmans-Green, London 1 (1906)
 R.C. Cammarata, Progress in Surface Science 46 (1994) 1–38.
 S. Cuenot, C. Frétigny, S. Demoustier-Champagne, B. Nysten, Physical Review
B: Condensed Matter 69 (2004) 165410.
 K. Kang, W. Cai, International Journal of Plasticity 26 (2010) 1387–1401.
 R.E. Miller, V.B. Shenoy, Nanotechnology 11 (2000) 139–147.
 H. Mehrez, S. Ciraci, Physical Review B: Condensed Matter 56 (1997)
 G. Wang, X. Feng, Applied Physics Letters 94 (2009) 141913.
 G. Huang, B. Svendsen, International Journal of Fracture 166 (2010) 173–178.
 X. Zheng, Y. Cao, B. Li, X. Feng, G. Wang, Nanotechnology 21 (2010) 205702.
 G. Ouyang, X.L. Li, X. Tan, G.W. Yang, Physical Review B: Condensed Matter 76
 B. Gong, Q. Chen, D. Wang, Materials Letters 67 (2012) 165–168.
 H. Masuda, K. Fukuda, Science 268 (1995) 1466–1468.
 D. Li, H. Zhou, I. Honma, Nat. Mater. 3 (2004) 65–72.
 H.L. Duan, J. Wang, B.L. Karihaloo, Z.P. Huang, Acta Materialia 54 (2006)
 G. Ouyang, G Yang, C. Sun, W. Zhu, Small 4 (2008) 1359–1362.
 X. Feng, R. Xia, X. Li, B. Li, Applied Physics Letters 94 (2009) 011916.
 W.X. Zhang, T.J. Wang, Applied Physics Letters 90 (2007) 063104.
 A.M. Hodge, J. Biener, J.R. Hayes, P.M. Bythrow, C.A. Volkert, A.V. Hamza, Acta
Materialia 55 (2007) 1343–1349.
 M. Hakamada, M. Mabuchi, Scripta Materialia 56 (2007) 1003–1006.
 J.R. Greer, J Th, M. De Hosson, Progress in Materials Science 56 (2011) 654–724.
 W.X. Zhang, T.J. Wang, X. Chen, International Journal of Plasticity 26 (2010)
 Q. Chen, N. Pugno, EPL 97 (2012) 26002.
 Q. Chen, N. Pugno, EPL 98 (2012) 16005.
 Q. Chen, N. Pugno, European Journal of Mechanics—A/Solids 37 (2013) 248–255.
 A. Garcia, D. Sen, M.J. Buehler, Metallurgical and Materials Transactions
A: Physical Metallurgy and Materials Science 42 (2011) 3889–3897.
 J.L. Zang, Y.-P. Zhao, International Journal of Engineering Science 61 (2012) 156–170.
 J. He, C.M. Lilley, Nano Letters 8 (2008) 1798–1802.
 V.B. Shenoy, Physical Review B: Condensed Matter 71 (2005) 094104.
 G-F. Wang, X.Q. Feng, Applied Physics Letters 90 (2007) 231904.
 D.C.C. Lam, F. Yang, A.C.M. Chong, J. Wang, P. Tong, Journal of the Mechanics
and Physics of Solids 51 (2003) 1477–1508.
 Z.Q. Wang, Y-P. Zhao, Z.P. Huang, International Journal of Engineering Science
48 (2010) 140–150.
 Z. Wang, Y. Zhao, Acta Mechanica Solida Sinica 22 (2009) 630–643.
 L.J. Gibson, M.F. Ashby., Cellular Solids: Structure and Properties, second ed,
Cambridge University Press, Cambridge, 1997.
 F. Wang, S. Zhuang, J. Yu, Acta Mechanica Solida Sinica 34 (2002) 914–923